Presentation on theme: "Metal-Air Batteries: Types, Applications, and Challenges NPRE 498 Energy Storage Systems Marta Baginska 12.07.2011."— Presentation transcript:
Metal-Air Batteries: Types, Applications, and Challenges NPRE 498 Energy Storage Systems Marta Baginska 12.07.2011
Outline Introduction o Scope of the presentation: Where do metal-air batteries fit in? o General characteristics of metal-air batteries o Factors the affect performance o Air electrode requirements Zinc-Air Batteries o Characteristics o Chemistry o Types (primary and refuelable) Lithium-Air Batteries o Characteristics o Extent of rechargeability o Current issues and challenges Conclusions
Current Energy Outlook Advanced electronic equipment has been developing at a rapid pace, resulting in an ever-increasing demand for high energy density and high power density power sources. Li-ion technologies are currently the hope for meeting many of these demands, i.e, electric vehicles. The energy density of Li-ion batteries is limited by the intercalation chemistry of the electrodes.
Current Battery Outlook Metal-air batteries have garnered much attention recently as a possible alternative, due to their extremely high energy density compared to that of other rechargeable batteries:
Metal-Air Battery Concept This high specific energy density is a result of the coupling of a reactive metal anode to an air electrode, thus providing a battery with an inexhaustible cathode reactant.
Metal-Air Batteries AdvantagesDisadvantages High energy density Dependent on environmental conditions: - Drying out limits shelf life once opened to air - Electrolyte flooding limits power output Flat discharge voltage Long shelf life (dry storage) Non toxic (on metal use basis)Limited power density Low cost (on metal use basis)Limited operating temperature range The major advantages and disadvantages are summarized below..
Metal-Air Battery Properties Typically divided into two categories based on electrolyte type: (i) aqueous or (ii) non-aqueous. Can be primary, secondary, or ‘refuelable’. A variety of metals have been considered for use: Metal/air battery Calculated OCV, V Theoretical specific energy, Wh/kg Incl. oxygenExcluding oxygen Li/O 2 2.91520011140 Na/O 2 1.9416772260 Ca/O 2 3.1229904180 Mg/O 2 2.9327896462 Zn/O 2 1.6510901350
Factors That Affect Performance Most metals are unstable in water and react with the electrolyte to corrode the metal, resulting in self-discharge. Electrode polarization: sharp voltage drop-off with increasing current because of oxygen diffusion limitations, making metal- air batteries more suited to low-power applications rather than high-power. Electrode carbonation: Absorption of CO 2 (since the cell is an open system), results in crystallization of carbonate in the air electrode, clogging pores and decreasing performance. Water transpiration: Movement of water vapor either into or out of the cell. o Excessive water loss can lead to drying of the cell and premature failure. o Excessive gain of water can dilute the electrolyte.
Air Electrode Requirements Cathode must be able to sustain an oxygen reduction reaction (and oxidation if battery is rechargeable). Cathode must be highly porous. Catalysts are typically incorporated into the carbon layer.
Outline Introduction o Scope of the presentation o General characteristics of metal-air batteries o Factors the affect performance o Air electrode requirements Zinc-Air Batteries o Characteristics o Chemistry o Types (Primary and ‘rechargeable’) Lithium-Air Batteries o Characteristics o Extent of rechargeability o Current issues and challenges Conclusions and perspective
History of Metal-Air Batteries Zinc was the first metal implemented in metal-air batteries. Zinc is stable in aqueous and alkaline electrolytes without significant corrosion. c
Zn-Air Applications Commercial, primary Zn-air batteries have been used for many years: o Initially used as large batteries for applications such as railroad signaling, remote communications, and ocean navigational units requiring long term, low rate discharge. o With the development of thin electrodes, used in small, high capacity primary cells, such as for hearing aids, small electronics, and medical devices.
Are Zn-Air Cells Rechargeable? Not really. Not electrically anyhow… why? Problems of dendrite formation, non-uniform zinc deposition, limited solubility of the reaction products.. One of the decomposition products of zincate is ZnO, a white solid powder that acts as an insulator. But they are refuelable!
Refuelable Zn-Air Cells Santa Barbara Municipal Transit District “Downtown Waterfront Electric Shuttle” Powered by refuelable Zn-air cells. Road test underscored potential of such vehicles. o 250 mile range between refueling o Rapid refueling (10 minutes) o Highway safe acceleration
Refuelable Zn-Air Cells
Refuelable Zn-Air cells
Update 7 Years Later.. Despite this novel design and successful roadside demonstration, why have battery-electric busses failed to achieve meaningful market presentation ? The busses suffered from: o Reliability issues: Inconsistent performance Sensitivity to temperature o Performance issues: Marginal hill climbing o Life-cycle cost issues: Battery was maintenance intensive
Zn-Air Summary Primary Zn-air batteries have been very successful commercially. To take the technology to the next level, i.e, developing secondary, electrically rechargeable batteries, or using Zn-air technologies for vehicle propulsion, significant challenges must still be overcome: o Understand the chemistry of the zincate anion in an alkaline solution. o Develop stable bifunctional catalysts for both the oxygen reduction reaction and oxygen evolution reaction. o The air electrode should be optimized to reduce internal resistance.
Outline Introduction o Scope of the presentation: Where do metal-air batteries fit in? o General characteristics of metal-air batteries o Factors the affect performance o Air electrode requirements Zinc-Air Batteries o Characteristics o Chemistry o Types (Primary and ‘rechargeable’) Lithium-Air Batteries o Characteristics o Extent of rechargeability o Current issues and challenges Conclusions and Future Perspective
Why Li-Air? Extremely high specific capacity of Li anode material ( 3842 mAh g ‑ 1 for lithium, vs. 815 mAh g -1 for Zinc) The couple voltage of Li-O 2 in alkaline electrolytes is 2.91 V (compared to 1.65 for Zn-O 2 ) The Li-air battery, when fully developed, could have practical specific energies of 1000-3000 Wh kg -1 Li-air cell IS electrically rechargeable, (far more so than the Zn- air battery.)
Currently, Li-air batteries are still in the opening development stage, and their actual parameters fall far short of the theoretical values. Li-air cell capacity fades twice as fast after 50 cycles (compared to 25% capacity fade after 300 cycles for an ordinary Li-ion cell). Not So Fast Though… Li-airLi-ion Specific Energy 362 Wh kg -1 (lab model!)200 Wh kg -1 Specific Power ~ 0.46 mW g -1 42 mW g -1 (when discharged at 0.2C)
Li-Air Cell Architectures
How are Li-air cells rechargeable? In 2006, Bruce et al. demonstrated that Li 2 O 2 is formed on charging and decomposes according to the reaction below: Secondary Li-Air Cells Li (s) → Li + + e - (anode reaction) Li + + ½O 2 + e - → ½Li 2 O 2 (cathode reaction) Li + + e - + ¼O 2 → ½Li 2 O (cathode reaction) Li 2 O 2 → O 2 + 2Li + + 2e -
Electrocatalysts Critical challenges that limit the practical use of this technology currently include: o Sluggish oxygen reduction reaction (ORR) kinetics (during discharging). o Sluggish oxygen evolution reaction (OER) kinetics (during charging). Currently, these reactions are too slow for practical applications in electric vehicles. As a result, a lot of effort has been put into developing effective, bifunctional, electrocatalysts for the ORR and OER. OER ORR
Recent Advances in Electrocatalysts (1) In a recently published paper (2010), Lu et al. have shown, Pt/Au nanoparticles applied to a carbon cathode were shown to strongly enhance the kinetics of the ORR and OER, with Au enhancing the ORR, and Pt enhancing the OER. Li-air batteries built with this catalyst boasted the highest cell efficiency reported for a Li-air cell with an efficiency of 77%.
Recent Advances in Electrocatalysts (2) Bruce et al. has also been developing catalysts to improve ORR and OER kinetics. They have been particularly successful with various nano-structured manganese oxide catalysts.
Air Cathode Challenges Cathode reaction delivers most of the energy, and because most of the cell voltage drop occurs at the air cathode. It is thought that non-aqueous Li-air energy falls far short of the theoretical values because the discharge terminated well before all of the pores in the air electrode are filled with Lithium oxides. How can this be combatted? o Develop new cathode materials that can accommodate large amounts of oxides. o Including additives that improve the solubility of the precipitates. o Develop catalysts that alter the morphology of lithium-oxide deposits.
Li-Metal Anode Challenges Lithium metal anodes are the anodes of choice for Li-air cells because of their high energy density compared to Lithium intercalation anodes. Implementation of Li-metal anodes is associated with: o Dendrite formation (which can lead to dangerous battery shorts) o Electrolyte incompatibility (which results in resistive films forming on the anode surface) How to combat this? Incorporating a solid polymer electrolyte, o Inert to Lithium metal o Conducts Li-ions o Prevents dendrite formation
Electrolyte Challenges AqueousNon-Aqueous Li-battery grade electrolytes are quite volatile! Solutions? Developing hydrophobic electrolytes with low volatility Developing compound electrolytes (i.e, electrolytes with multiple layers with different properties) Major challenge is related to the prevention of water and oxygen access to the Li-metal. Solutions? One such potential solution was the LiSICON porous glass concept, which makes Li-metal stable in water Durability and manufacturing the film in large quantities may become an additional challenge.
Summary & Conclusions Metal-air batteries offer great benefits if they can be harnessed to their fullest potential. Recap of Zn-air vs. Li-air: Important to continue development of both systems! Zn-airLi-air Stable towards moisture, can be assembled outside of glovebox. Not moisture-stable, increasing cost and manufacturing complexity. Zinc metal and aqueous electrolytes are inexpensive Lithium and non-aqueous electrolytes are costly Technology is closer to or already in practical applications. Still in research phase Poor reversibility of reactionsReversible reactions (and improving!) Low operating potentialHighest operating potential
References  J. Lee, S. Tai Kim, R. Cao, N. Choi, M. Liu, K.T. Lee, J. Cho, Advanced Energy Materials 2011, 1, 34-50.  R.P. Hamlen, T.B. Atwater, in Handbook of Batteries, Mcgraw-hill 2004, 38.1- 38.53.  K.M. Abraham, Ecs 2008, 67-71.  W. Qu, 'The Development of Materials and Components for Metal-air Battery Applications at NRC', 2011. 'Powering Future Vehicles with the Refuelable Zinc/Air Battery', Lawrence Livermore National Laboratory,, 1995. P. Griffith, 'Don't Give up on the Battery-Electric Bus Just Yet...' Electric Bus Workshop, 2002.  A. Kraytsberg, Y. Ein-Eli, Journal of Power Sources 2011, 196, 886-893.  T. Ogasawara, A. Débart, M. Holzapfel, P. Novák, P.G. Bruce, J. Am. Chem. Soc. 2006, 128, 1390-1393.  S.J. Visco, B.D. Katz, Y.S. Nimon, L.C. De Jonghe, Protected Active Metal Electrode and Battery Cell Structures with Non-aqueous Interlayer Architecture, n.d., U.S. Patent 7282295.  M. Jacoby, Chemical & Engineering News 2010, 29-31.  A. Débart, J. Bao, G. Armstrong, P.G. Bruce, Journal of Power Sources 2007, 174, 1177-1182.